#------------------------------------------------------------------------------
#$Date: 2016-02-20 00:18:51 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176760 $
#$URL: svn://www.crystallography.net/cod/cif/2/01/44/2014429.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2014429
loop_
_publ_author_name
'Emme, Holger'
'Huppertz, Hubert'
_publ_section_title
;
 High-pressure synthesis of ν-DyBO₃
;
_journal_issue                   12
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              i117
_journal_page_last               i119
_journal_paper_doi               10.1107/S0108270104024205
_journal_volume                  60
_journal_year                    2004
_chemical_formula_iupac          'Dy B O3'
_chemical_formula_moiety         'B Dy O3'
_chemical_formula_sum            'B Dy O3'
_chemical_formula_weight         221.31
_chemical_name_common            'ν-dysprosium orthoborate'
_chemical_name_systematic
;
Dysprosium borate
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                92.52(3)
_cell_angle_beta                 107.65(3)
_cell_angle_gamma                108.29(3)
_cell_formula_units_Z            4
_cell_length_a                   6.1463(12)
_cell_length_b                   6.3856(13)
_cell_length_c                   6.3894(13)
_cell_measurement_reflns_used    3498
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      37.785
_cell_measurement_theta_min      3.134
_cell_volume                     224.19(10)
_computing_cell_refinement       'HKL SCALEPACK (Otwinowski & Minor, 1997)'
_computing_data_collection       'COLLECT (Nonius, 1998)'
_computing_data_reduction
'HKL DENZO (Otwinowski & Minor, 1997) and SCALEPACK'
_computing_molecular_graphics    'DIAMOND (Brandenburg & Berndt, 1999)'
_computing_publication_material  'enCIFer (Allen et al., 2004) and SHELXL97'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      200(2)
_diffrn_detector_area_resol_mean 9
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Nonius KappaCCD area-detector'
_diffrn_measurement_method       '95 mm CCD camera on κ-Goniostat'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0460
_diffrn_reflns_av_sigmaI/netI    0.0418
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            6397
_diffrn_reflns_theta_full        32.48
_diffrn_reflns_theta_max         32.48
_diffrn_reflns_theta_min         3.39
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    33.014
_exptl_absorpt_correction_T_max  0.75953
_exptl_absorpt_correction_T_min  0.43202
_exptl_absorpt_correction_type   '\y scan'
_exptl_absorpt_process_details   '(XPREP; Siemens, 1996)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    6.557
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       rod
_exptl_crystal_F_000             380
_exptl_crystal_size_max          0.027
_exptl_crystal_size_mid          0.018
_exptl_crystal_size_min          0.008
_refine_diff_density_max         2.532
_refine_diff_density_min         -2.721
_refine_ls_extinction_coef       0.0101(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL97 (Sheldrick, 1997)'
_refine_ls_goodness_of_fit_ref   1.147
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     92
_refine_ls_number_reflns         1623
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.147
_refine_ls_R_factor_all          0.0293
_refine_ls_R_factor_gt           0.0218
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0081P)²+0.5392P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0498
_refine_ls_wR_factor_ref         0.0513
_reflns_number_gt                1446
_reflns_number_total             1623
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            bc1055.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_cell_volume        224.20(10)
_cod_database_code               2014429
_cod_database_fobs_code          2014429
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_type_symbol
Dy1 0.94025(4) 0.71995(4) 0.81700(3) 0.00547(8) Uani d . 1 . . Dy
Dy2 0.55505(4) 0.84498(4) 0.27142(3) 0.00615(8) Uani d . 1 . . Dy
O1 0.5894(6) 0.8664(6) 0.6455(6) 0.0079(7) Uani d . 1 . . O
O2 0.5327(6) 0.5246(6) 0.7716(6) 0.0099(7) Uani d . 1 . . O
O4 1.1206(6) 0.6610(6) 0.2034(6) 0.0073(6) Uani d . 1 . . O
O3 0.3484(6) 0.7820(6) 0.8760(6) 0.0085(7) Uani d . 1 . . O
O5 0.8722(6) 0.8830(6) 0.1289(5) 0.0068(6) Uani d . 1 . . O
O6 0.9555(8) 0.7643(7) 0.4773(6) 0.0155(8) Uani d . 1 . . O
B1 0.4778(10) 0.7132(9) 0.7601(9) 0.0065(9) Uani d . 1 . . B
B2 0.9897(10) 0.7686(9) 0.2815(9) 0.0062(9) Uani d . 1 . . B
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O6 Dy1 O3 . 1_655 79.20(14) no
O6 Dy1 O4 . 2_766 98.96(14) no
O3 Dy1 O4 1_655 2_766 87.93(12) no
O6 Dy1 O2 . . 106.20(15) no
O3 Dy1 O2 1_655 . 158.74(13) no
O4 Dy1 O2 2_766 . 70.99(12) no
O6 Dy1 O5 . 2_776 80.44(14) no
O3 Dy1 O5 1_655 2_776 74.91(12) no
O4 Dy1 O5 2_766 2_776 162.68(12) no
O2 Dy1 O5 . 2_776 125.98(12) no
O6 Dy1 O5 . 1_556 143.47(13) no
O3 Dy1 O5 1_655 1_556 112.85(12) no
O4 Dy1 O5 2_766 1_556 115.28(12) no
O2 Dy1 O5 . 1_556 75.38(13) no
O5 Dy1 O5 2_776 1_556 70.66(14) no
O6 Dy1 O4 . 1_556 151.56(13) no
O3 Dy1 O4 1_655 1_556 73.03(12) no
O4 Dy1 O4 2_766 1_556 74.30(13) no
O2 Dy1 O4 . 1_556 97.74(13) no
O5 Dy1 O4 2_776 1_556 97.91(12) no
O5 Dy1 O4 1_556 1_556 57.50(11) no
O6 Dy1 O1 . . 76.70(13) no
O3 Dy1 O1 1_655 . 143.95(13) no
O4 Dy1 O1 2_766 . 121.94(12) no
O2 Dy1 O1 . . 56.02(13) no
O5 Dy1 O1 2_776 . 74.96(12) no
O5 Dy1 O1 1_556 . 74.60(11) no
O4 Dy1 O1 1_556 . 130.64(11) no
O6 Dy1 B1 . . 100.34(15) no
O3 Dy1 B1 1_655 . 171.62(15) no
O4 Dy1 B1 2_766 . 100.38(15) no
O2 Dy1 B1 . . 29.44(14) no
O5 Dy1 B1 2_776 . 96.74(14) no
O5 Dy1 B1 1_556 . 62.69(13) no
O4 Dy1 B1 1_556 . 108.03(14) no
O1 Dy1 B1 . . 29.94(14) no
O6 Dy1 B2 . 1_556 166.88(16) no
O3 Dy1 B2 1_655 1_556 95.39(14) no
O4 Dy1 B2 2_766 1_556 92.73(14) no
O2 Dy1 B2 . 1_556 83.18(15) no
O5 Dy1 B2 2_776 1_556 86.63(14) no
O5 Dy1 B2 1_556 1_556 29.07(13) no
O4 Dy1 B2 1_556 1_556 28.78(13) no
O1 Dy1 B2 . 1_556 102.13(13) no
B1 Dy1 B2 . 1_556 83.26(15) no
O6 Dy1 Dy2 . 2_776 58.44(12) no
O3 Dy1 Dy2 1_655 2_776 43.85(10) no
O4 Dy1 Dy2 2_766 2_776 126.88(9) no
O2 Dy1 Dy2 . 2_776 155.69(10) no
O5 Dy1 Dy2 2_776 2_776 38.73(8) no
O5 Dy1 Dy2 1_556 2_776 105.35(9) no
O4 Dy1 Dy2 1_556 2_776 102.99(9) no
O1 Dy1 Dy2 . 2_776 100.25(9) no
B1 Dy1 Dy2 . 2_776 128.92(12) no
B2 Dy1 Dy2 1_556 2_776 109.52(12) no
O6 Dy1 Dy2 . 2_666 103.85(12) no
O3 Dy1 Dy2 1_655 2_666 126.19(9) no
O4 Dy1 Dy2 2_766 2_666 38.25(8) no
O2 Dy1 Dy2 . 2_666 32.83(9) no
O5 Dy1 Dy2 2_776 2_666 158.81(8) no
O5 Dy1 Dy2 1_556 2_666 96.11(9) no
O4 Dy1 Dy2 1_556 2_666 87.97(9) no
O1 Dy1 Dy2 . 2_666 85.73(9) no
B1 Dy1 Dy2 . 2_666 62.13(12) no
B2 Dy1 Dy2 1_556 2_666 89.02(12) no
Dy2 Dy1 Dy2 2_776 2_666 158.539(13) no
O2 Dy2 O1 2_666 . 92.83(13) no
O2 Dy2 O5 2_666 . 89.63(13) no
O1 Dy2 O5 . . 126.00(12) no
O2 Dy2 O1 2_666 2_676 143.27(13) no
O1 Dy2 O1 . 2_676 72.59(14) no
O5 Dy2 O1 . 2_676 126.41(13) no
O2 Dy2 O3 2_666 1_554 84.30(14) no
O1 Dy2 O3 . 1_554 156.42(12) no
O5 Dy2 O3 . 1_554 77.47(11) no
O1 Dy2 O3 2_676 1_554 95.94(12) no
O2 Dy2 O4 2_666 1_455 70.74(12) no
O1 Dy2 O4 . 1_455 84.78(12) no
O5 Dy2 O4 . 1_455 145.04(11) no
O1 Dy2 O4 2_676 1_455 74.41(12) no
O3 Dy2 O4 1_554 1_455 72.16(12) no
O2 Dy2 O3 2_666 2_676 151.17(12) no
O1 Dy2 O3 . 2_676 115.80(12) no
O5 Dy2 O3 . 2_676 71.37(12) no
O1 Dy2 O3 2_676 2_676 56.71(11) no
O3 Dy2 O3 1_554 2_676 70.78(14) no
O4 Dy2 O3 1_455 2_676 112.98(11) no
O2 Dy2 O6 2_666 . 72.06(14) no
O1 Dy2 O6 . . 73.92(12) no
O5 Dy2 O6 . . 55.81(12) no
O1 Dy2 O6 2_676 . 131.17(12) no
O3 Dy2 O6 1_554 . 126.53(11) no
O4 Dy2 O6 1_455 . 135.73(13) no
O3 Dy2 O6 2_676 . 111.21(13) no
O2 Dy2 B2 2_666 . 73.33(14) no
O1 Dy2 B2 . . 101.50(14) no
O5 Dy2 B2 . . 29.43(14) no
O1 Dy2 B2 2_676 . 141.65(14) no
O3 Dy2 B2 1_554 . 100.06(13) no
O4 Dy2 B2 1_455 . 143.79(13) no
O3 Dy2 B2 2_676 . 96.45(14) no
O6 Dy2 B2 . . 27.76(13) no
O2 Dy2 B1 2_666 2_676 163.07(14) no
O1 Dy2 B1 . 2_676 93.84(14) no
O5 Dy2 B1 . 2_676 98.94(14) no
O1 Dy2 B1 2_676 2_676 28.20(13) no
O3 Dy2 B1 1_554 2_676 83.37(14) no
O4 Dy2 B1 1_455 2_676 94.39(13) no
O3 Dy2 B1 2_676 2_676 28.52(12) no
O6 Dy2 B1 . 2_676 124.78(14) no
B2 Dy2 B1 . 2_676 120.33(16) no
O2 Dy2 Dy1 2_666 2_776 129.08(9) no
O1 Dy2 Dy1 . 2_776 111.51(10) no
O5 Dy2 Dy1 . 2_776 39.73(9) no
O1 Dy2 Dy1 2_676 2_776 87.54(9) no
O3 Dy2 Dy1 1_554 2_776 87.89(9) no
O4 Dy2 Dy1 1_455 2_776 151.12(9) no
O3 Dy2 Dy1 2_676 2_776 38.86(7) no
O6 Dy2 Dy1 . 2_776 72.99(10) no
B2 Dy2 Dy1 . 2_776 58.72(12) no
B1 Dy2 Dy1 2_676 2_776 61.96(11) no
O2 Dy2 Dy2 2_666 2_676 122.24(10) no
O1 Dy2 Dy2 . 2_676 36.81(9) no
O5 Dy2 Dy2 . 2_676 137.13(9) no
O1 Dy2 Dy2 2_676 2_676 35.78(8) no
O3 Dy2 Dy2 1_554 2_676 128.80(8) no
O4 Dy2 Dy2 1_455 2_676 77.03(8) no
O3 Dy2 Dy2 2_676 2_676 85.53(7) no
O6 Dy2 Dy2 . 2_676 104.10(8) no
B2 Dy2 Dy2 . 2_676 127.92(11) no
B1 Dy2 Dy2 2_676 2_676 59.18(11) no
Dy1 Dy2 Dy2 2_776 2_676 101.41(3) no
B1 O1 Dy2 . . 131.1(3) no
B1 O1 Dy2 . 2_676 97.2(3) no
Dy2 O1 Dy2 . 2_676 107.41(14) no
B1 O1 Dy1 . . 81.5(3) no
Dy2 O1 Dy1 . . 103.23(12) no
Dy2 O1 Dy1 2_676 . 139.57(15) no
B1 O2 Dy2 . 2_666 154.6(3) no
B1 O2 Dy1 . . 91.9(3) no
Dy2 O2 Dy1 2_666 . 112.55(14) no
B2 O4 Dy1 . 2_766 125.6(3) no
B2 O4 Dy2 . 1_655 120.8(3) no
Dy1 O4 Dy2 2_766 1_655 105.53(13) no
B2 O4 Dy1 . 1_554 91.9(3) no
Dy1 O4 Dy1 2_766 1_554 105.70(13) no
Dy2 O4 Dy1 1_655 1_554 101.72(13) no
B1 O3 Dy1 . 1_455 135.2(3) no
B1 O3 Dy2 . 1_556 111.5(3) no
Dy1 O3 Dy2 1_455 1_556 107.77(13) no
B1 O3 Dy2 . 2_676 89.5(3) no
Dy1 O3 Dy2 1_455 2_676 97.29(13) no
Dy2 O3 Dy2 1_556 2_676 109.22(14) no
B2 O5 Dy2 . . 95.5(3) no
B2 O5 Dy1 . 2_776 116.6(3) no
Dy2 O5 Dy1 . 2_776 101.54(12) no
B2 O5 Dy1 . 1_554 94.3(2) no
Dy2 O5 Dy1 . 1_554 138.82(16) no
Dy1 O5 Dy1 2_776 1_554 109.34(14) no
B2 O6 Dy1 . . 169.8(3) no
B2 O6 Dy2 . . 84.9(3) no
Dy1 O6 Dy2 . . 104.38(14) no
O2 B1 O1 . . 116.4(4) yes
O2 B1 O3 . . 126.4(5) yes
O1 B1 O3 . . 116.5(4) yes
O2 B1 Dy1 . . 58.7(2) no
O1 B1 Dy1 . . 68.6(2) no
O3 B1 Dy1 . . 140.1(3) no
O2 B1 Dy2 . 2_676 169.8(4) no
O1 B1 Dy2 . 2_676 54.6(2) no
O3 B1 Dy2 . 2_676 62.0(3) no
Dy1 B1 Dy2 . 2_676 111.29(19) no
O6 B2 O4 . . 127.0(5) yes
O6 B2 O5 . . 117.9(4) yes
O4 B2 O5 . . 114.9(4) yes
O6 B2 Dy2 . . 67.3(3) no
O4 B2 Dy2 . . 153.4(3) no
O5 B2 Dy2 . . 55.0(2) no
O6 B2 Dy1 . 1_554 166.2(4) no
O4 B2 Dy1 . 1_554 59.3(2) no
O5 B2 Dy1 . 1_554 56.6(2) no
Dy2 B2 Dy1 . 1_554 102.04(17) no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Dy1 O6 . 2.227(4) yes
Dy1 O3 1_655 2.320(3) yes
Dy1 O4 2_766 2.334(4) yes
Dy1 O2 . 2.341(4) yes
Dy1 O5 2_776 2.393(4) yes
Dy1 O5 1_556 2.414(3) yes
Dy1 O4 1_556 2.480(4) yes
Dy1 O1 . 2.578(4) yes
Dy1 B1 . 2.740(5) no
Dy1 B2 1_556 2.882(5) no
Dy1 Dy2 2_776 3.6678(13) no
Dy1 Dy2 2_666 3.8061(16) no
Dy2 O2 2_666 2.234(4) yes
Dy2 O1 . 2.329(3) yes
Dy2 O5 . 2.342(3) yes
Dy2 O1 2_676 2.386(3) yes
Dy2 O3 1_554 2.409(4) yes
Dy2 O4 1_455 2.446(4) yes
Dy2 O3 2_676 2.562(4) yes
Dy2 O6 . 2.635(4) yes
Dy2 B2 . 2.845(5) no
Dy2 B1 2_676 2.903(6) no
Dy2 Dy1 2_776 3.6678(13) no
Dy2 Dy2 2_676 3.8000(11) no
B1 O1 . 1.382(7) yes
B1 O2 . 1.347(6) yes
B1 O3 . 1.386(6) yes
B2 O4 . 1.388(6) yes
B2 O5 . 1.405(6) yes
B2 O6 . 1.330(6) yes
B1 Dy2 2_676 2.903(6) no
B2 Dy1 1_554 2.882(5) no
O1 Dy2 2_676 2.386(3) no
O2 Dy2 2_666 2.234(4) no
O4 Dy1 2_766 2.334(4) no
O4 Dy2 1_655 2.446(4) no
O4 Dy1 1_554 2.480(4) no
O3 Dy1 1_455 2.320(3) no
O3 Dy2 1_556 2.409(3) no
O3 Dy2 2_676 2.562(4) no
O5 Dy1 2_776 2.393(4) no
O5 Dy1 1_554 2.414(3) no
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
O2 Dy2 O1 B1 2_666 . -29.1(4) no
O5 Dy2 O1 B1 . . -120.7(4) no
O1 Dy2 O1 B1 2_676 . 116.5(4) no
O3 Dy2 O1 B1 1_554 . 53.1(5) no
O4 Dy2 O1 B1 1_455 . 41.2(4) no
O3 Dy2 O1 B1 2_676 . 154.3(4) no
O6 Dy2 O1 B1 . . -99.6(4) no
B2 Dy2 O1 B1 . . -102.7(4) no
B1 Dy2 O1 B1 2_676 . 135.3(3) no
Dy1 Dy2 O1 B1 2_776 . -163.4(4) no
Dy2 Dy2 O1 B1 2_676 . 116.5(4) no
O2 Dy2 O1 Dy2 2_666 2_676 -145.64(14) no
O5 Dy2 O1 Dy2 . 2_676 122.75(15) no
O1 Dy2 O1 Dy2 2_676 2_676 0.0 no
O3 Dy2 O1 Dy2 1_554 2_676 -63.4(4) no
O4 Dy2 O1 Dy2 1_455 2_676 -75.28(14) no
O3 Dy2 O1 Dy2 2_676 2_676 37.76(17) no
O6 Dy2 O1 Dy2 . 2_676 143.94(17) no
B2 Dy2 O1 Dy2 . 2_676 140.80(15) no
B1 Dy2 O1 Dy2 2_676 2_676 18.79(16) no
Dy1 Dy2 O1 Dy2 2_776 2_676 80.10(13) no
O2 Dy2 O1 Dy1 2_666 . 61.07(14) no
O5 Dy2 O1 Dy1 . . -30.5(2) no
O1 Dy2 O1 Dy1 2_676 . -153.3(2) no
O3 Dy2 O1 Dy1 1_554 . 143.3(3) no
O4 Dy2 O1 Dy1 1_455 . 131.43(14) no
O3 Dy2 O1 Dy1 2_676 . -115.53(13) no
O6 Dy2 O1 Dy1 . . -9.35(12) no
B2 Dy2 O1 Dy1 . . -12.49(17) no
B1 Dy2 O1 Dy1 2_676 . -134.50(15) no
Dy1 Dy2 O1 Dy1 2_776 . -73.19(12) no
Dy2 Dy2 O1 Dy1 2_676 . -153.3(2) no
O6 Dy1 O1 B1 . . 141.3(3) no
O3 Dy1 O1 B1 1_655 . -169.4(3) no
O4 Dy1 O1 B1 2_766 . 48.9(3) no
O2 Dy1 O1 B1 . . 20.9(2) no
O5 Dy1 O1 B1 2_776 . -135.2(3) no
O5 Dy1 O1 B1 1_556 . -61.6(3) no
O4 Dy1 O1 B1 1_556 . -47.7(3) no
B2 Dy1 O1 B1 1_556 . -52.1(3) no
Dy2 Dy1 O1 B1 2_776 . -164.9(2) no
Dy2 Dy1 O1 B1 2_666 . 35.9(2) no
O6 Dy1 O1 Dy2 . . 10.94(15) no
O3 Dy1 O1 Dy2 1_655 . 60.3(2) no
O4 Dy1 O1 Dy2 2_766 . -81.43(17) no
O2 Dy1 O1 Dy2 . . -109.40(17) no
O5 Dy1 O1 Dy2 2_776 . 94.43(15) no
O5 Dy1 O1 Dy2 1_556 . 168.07(16) no
O4 Dy1 O1 Dy2 1_556 . -178.02(12) no
B1 Dy1 O1 Dy2 . . -130.3(3) no
B2 Dy1 O1 Dy2 1_556 . 177.54(14) no
Dy2 Dy1 O1 Dy2 2_776 . 64.82(12) no
Dy2 Dy1 O1 Dy2 2_666 . -94.39(12) no
O6 Dy1 O1 Dy2 . 2_676 -127.7(3) no
O3 Dy1 O1 Dy2 1_655 2_676 -78.3(3) no
O4 Dy1 O1 Dy2 2_766 2_676 140.0(2) no
O2 Dy1 O1 Dy2 . 2_676 112.0(3) no
O5 Dy1 O1 Dy2 2_776 2_676 -44.2(2) no
O5 Dy1 O1 Dy2 1_556 2_676 29.5(2) no
O4 Dy1 O1 Dy2 1_556 2_676 43.4(3) no
B1 Dy1 O1 Dy2 . 2_676 91.1(3) no
B2 Dy1 O1 Dy2 1_556 2_676 38.9(3) no
Dy2 Dy1 O1 Dy2 2_776 2_676 -73.8(2) no
Dy2 Dy1 O1 Dy2 2_666 2_676 127.0(2) no
O6 Dy1 O2 B1 . . -82.3(3) no
O3 Dy1 O2 B1 1_655 . 175.7(3) no
O4 Dy1 O2 B1 2_766 . -176.4(3) no
O5 Dy1 O2 B1 2_776 . 7.6(3) no
O5 Dy1 O2 B1 1_556 . 59.8(3) no
O4 Dy1 O2 B1 1_556 . 113.3(3) no
O1 Dy1 O2 B1 . . -21.3(3) no
B2 Dy1 O2 B1 1_556 . 88.4(3) no
Dy2 Dy1 O2 B1 2_776 . -35.2(4) no
Dy2 Dy1 O2 B1 2_666 . -172.8(4) no
O6 Dy1 O2 Dy2 . 2_666 90.54(19) no
O3 Dy1 O2 Dy2 1_655 2_666 -11.5(4) no
O4 Dy1 O2 Dy2 2_766 2_666 -3.56(13) no
O5 Dy1 O2 Dy2 2_776 2_666 -179.62(12) no
O5 Dy1 O2 Dy2 1_556 2_666 -127.38(19) no
O4 Dy1 O2 Dy2 1_556 2_666 -73.95(17) no
O1 Dy1 O2 Dy2 . 2_666 151.5(2) no
B1 Dy1 O2 Dy2 . 2_666 172.8(4) no
B2 Dy1 O2 Dy2 1_556 2_666 -98.83(18) no
Dy2 Dy1 O2 Dy2 2_776 2_666 137.63(13) no
O2 Dy2 O5 B2 2_666 . -55.1(3) no
O1 Dy2 O5 B2 . . 38.2(3) no
O1 Dy2 O5 B2 2_676 . 132.5(3) no
O3 Dy2 O5 B2 1_554 . -139.3(3) no
O4 Dy2 O5 B2 1_455 . -109.3(3) no
O3 Dy2 O5 B2 2_676 . 147.0(3) no
O6 Dy2 O5 B2 . . 13.3(3) no
B1 Dy2 O5 B2 2_676 . 139.6(3) no
Dy1 Dy2 O5 B2 2_776 . 118.7(3) no
Dy2 Dy2 O5 B2 2_676 . 85.9(3) no
O2 Dy2 O5 Dy1 2_666 2_776 -173.73(13) no
O1 Dy2 O5 Dy1 . 2_776 -80.50(17) no
O1 Dy2 O5 Dy1 2_676 2_776 13.88(18) no
O3 Dy2 O5 Dy1 1_554 2_776 102.03(14) no
O4 Dy2 O5 Dy1 1_455 2_776 132.05(18) no
O3 Dy2 O5 Dy1 2_676 2_776 28.34(11) no
O6 Dy2 O5 Dy1 . 2_776 -105.32(17) no
B2 Dy2 O5 Dy1 . 2_776 -118.7(3) no
B1 Dy2 O5 Dy1 2_676 2_776 20.92(15) no
Dy2 Dy2 O5 Dy1 2_676 2_776 -32.72(18) no
O2 Dy2 O5 Dy1 2_666 1_554 48.0(2) no
O1 Dy2 O5 Dy1 . 1_554 141.2(2) no
O1 Dy2 O5 Dy1 2_676 1_554 -124.4(2) no
O3 Dy2 O5 Dy1 1_554 1_554 -36.3(2) no
O4 Dy2 O5 Dy1 1_455 1_554 -6.3(4) no
O3 Dy2 O5 Dy1 2_676 1_554 -110.0(2) no
O6 Dy2 O5 Dy1 . 1_554 116.4(3) no
B2 Dy2 O5 Dy1 . 1_554 103.0(4) no
B1 Dy2 O5 Dy1 2_676 1_554 -117.4(2) no
Dy1 Dy2 O5 Dy1 2_776 1_554 -138.3(3) no
Dy2 Dy2 O5 Dy1 2_676 1_554 -171.03(13) no
O3 Dy1 O6 B2 1_655 . 42(2) no
O4 Dy1 O6 B2 2_766 . -44(2) no
O2 Dy1 O6 B2 . . -117(2) no
O5 Dy1 O6 B2 2_776 . 118(2) no
O5 Dy1 O6 B2 1_556 . 156(2) no
O4 Dy1 O6 B2 1_556 . 29(2) no
O1 Dy1 O6 B2 . . -165(2) no
B1 Dy1 O6 B2 . . -146(2) no
B2 Dy1 O6 B2 1_556 . 109(2) no
Dy2 Dy1 O6 B2 2_776 . 84(2) no
Dy2 Dy1 O6 B2 2_666 . -83(2) no
O3 Dy1 O6 Dy2 1_655 . -162.68(17) no
O4 Dy1 O6 Dy2 2_766 . 111.17(15) no
O2 Dy1 O6 Dy2 . . 38.48(18) no
O5 Dy1 O6 Dy2 2_776 . -86.37(15) no
O5 Dy1 O6 Dy2 1_556 . -48.7(3) no
O4 Dy1 O6 Dy2 1_556 . -175.33(19) no
O1 Dy1 O6 Dy2 . . -9.70(13) no
B1 Dy1 O6 Dy2 . . 8.81(18) no
B2 Dy1 O6 Dy2 1_556 . -96.1(6) no
Dy2 Dy1 O6 Dy2 2_776 . -120.79(16) no
Dy2 Dy1 O6 Dy2 2_666 . 72.43(13) no
O2 Dy2 O6 B2 2_666 . 88.1(3) no
O1 Dy2 O6 B2 . . -173.4(3) no
O5 Dy2 O6 B2 . . -14.1(3) no
O1 Dy2 O6 B2 2_676 . -125.1(3) no
O3 Dy2 O6 B2 1_554 . 19.8(4) no
O4 Dy2 O6 B2 1_455 . 122.2(3) no
O3 Dy2 O6 B2 2_676 . -61.4(3) no
B1 Dy2 O6 B2 2_676 . -90.0(3) no
Dy1 Dy2 O6 B2 2_776 . -54.2(3) no
Dy2 Dy2 O6 B2 2_676 . -152.1(3) no
O2 Dy2 O6 Dy1 2_666 . -87.59(18) no
O1 Dy2 O6 Dy1 . . 10.89(14) no
O5 Dy2 O6 Dy1 . . 170.2(2) no
O1 Dy2 O6 Dy1 2_676 . 59.1(2) no
O3 Dy2 O6 Dy1 1_554 . -155.88(13) no
O4 Dy2 O6 Dy1 1_455 . -53.5(2) no
O3 Dy2 O6 Dy1 2_676 . 122.86(15) no
B2 Dy2 O6 Dy1 . . -175.7(4) no
B1 Dy2 O6 Dy1 2_676 . 94.3(2) no
Dy1 Dy2 O6 Dy1 2_776 . 130.05(16) no
Dy2 Dy2 O6 Dy1 2_676 . 32.21(16) no
Dy2 O2 B1 O1 2_666 . -125.6(7) no
Dy1 O2 B1 O1 . . 38.8(4) no
Dy2 O2 B1 O3 2_666 . 63.8(10) no
Dy1 O2 B1 O3 . . -131.8(5) no
Dy2 O2 B1 Dy1 2_666 . -164.4(8) no
Dy2 O2 B1 Dy2 2_666 2_676 -153.0(14) no
Dy1 O2 B1 Dy2 . 2_676 11(2) no
Dy2 O1 B1 O2 . . 65.1(6) no
Dy2 O1 B1 O2 2_676 . -174.3(4) no
Dy1 O1 B1 O2 . . -35.1(4) no
Dy2 O1 B1 O3 . . -123.4(4) no
Dy2 O1 B1 O3 2_676 . -2.7(4) no
Dy1 O1 B1 O3 . . 136.5(4) no
Dy2 O1 B1 Dy1 . . 100.2(3) no
Dy2 O1 B1 Dy1 2_676 . -139.20(15) no
Dy2 O1 B1 Dy2 . 2_676 -120.6(4) no
Dy1 O1 B1 Dy2 . 2_676 139.20(15) no
Dy1 O3 B1 O2 1_455 . -87.0(6) no
Dy2 O3 B1 O2 1_556 . 62.6(6) no
Dy2 O3 B1 O2 2_676 . 173.1(5) no
Dy1 O3 B1 O1 1_455 . 102.4(5) no
Dy2 O3 B1 O1 1_556 . -108.0(4) no
Dy2 O3 B1 O1 2_676 . 2.5(4) no
Dy1 O3 B1 Dy1 1_455 . -169.9(3) no
Dy2 O3 B1 Dy1 1_556 . -20.3(7) no
Dy2 O3 B1 Dy1 2_676 . 90.2(5) no
Dy1 O3 B1 Dy2 1_455 2_676 99.9(4) no
Dy2 O3 B1 Dy2 1_556 2_676 -110.5(2) no
O6 Dy1 B1 O2 . . 104.7(3) no
O4 Dy1 B1 O2 2_766 . 3.5(3) no
O5 Dy1 B1 O2 2_776 . -173.8(3) no
O5 Dy1 B1 O2 1_556 . -109.7(3) no
O4 Dy1 B1 O2 1_556 . -73.2(3) no
O1 Dy1 B1 O2 . . 143.0(4) no
B2 Dy1 B1 O2 1_556 . -88.1(3) no
Dy2 Dy1 B1 O2 2_776 . 162.3(2) no
Dy2 Dy1 B1 O2 2_666 . 4.4(2) no
O6 Dy1 B1 O1 . . -38.2(3) no
O4 Dy1 B1 O1 2_766 . -139.5(2) no
O2 Dy1 B1 O1 . . -143.0(4) no
O5 Dy1 B1 O1 2_776 . 43.2(3) no
O5 Dy1 B1 O1 1_556 . 107.3(3) no
O4 Dy1 B1 O1 1_556 . 143.8(2) no
B2 Dy1 B1 O1 1_556 . 129.0(3) no
Dy2 Dy1 B1 O1 2_776 . 19.3(3) no
Dy2 Dy1 B1 O1 2_666 . -138.5(3) no
O6 Dy1 B1 O3 . . -144.4(6) no
O4 Dy1 B1 O3 2_766 . 114.4(6) no
O2 Dy1 B1 O3 . . 110.9(7) no
O5 Dy1 B1 O3 2_776 . -63.0(6) no
O5 Dy1 B1 O3 1_556 . 1.2(5) no
O4 Dy1 B1 O3 1_556 . 37.6(6) no
O1 Dy1 B1 O3 . . -106.2(7) no
B2 Dy1 B1 O3 1_556 . 22.8(6) no
Dy2 Dy1 B1 O3 2_776 . -86.9(6) no
Dy2 Dy1 B1 O3 2_666 . 115.3(6) no
O6 Dy1 B1 Dy2 . 2_676 -73.14(19) no
O4 Dy1 B1 Dy2 2_766 2_676 -174.34(15) no
O2 Dy1 B1 Dy2 . 2_676 -177.8(4) no
O5 Dy1 B1 Dy2 2_776 2_676 8.33(18) no
O5 Dy1 B1 Dy2 1_556 2_676 72.46(17) no
O4 Dy1 B1 Dy2 1_556 2_676 108.94(18) no
O1 Dy1 B1 Dy2 . 2_676 -34.89(19) no
B2 Dy1 B1 Dy2 1_556 2_676 94.11(18) no
Dy2 Dy1 B1 Dy2 2_776 2_676 -15.6(2) no
Dy2 Dy1 B1 Dy2 2_666 2_676 -173.4(2) no
Dy1 O6 B2 O4 . . 2(3) no
Dy2 O6 B2 O4 . . -153.9(5) no
Dy1 O6 B2 O5 . . 178.3(19) no
Dy2 O6 B2 O5 . . 22.3(4) no
Dy1 O6 B2 Dy2 . . 156(2) no
Dy1 O6 B2 Dy1 . 1_554 115(2) no
Dy2 O6 B2 Dy1 . 1_554 -40.7(16) no
Dy1 O4 B2 O6 2_766 . 54.4(7) no
Dy2 O4 B2 O6 1_655 . -89.9(6) no
Dy1 O4 B2 O6 1_554 . 165.3(5) no
Dy1 O4 B2 O5 2_766 . -122.0(4) no
Dy2 O4 B2 O5 1_655 . 93.8(4) no
Dy1 O4 B2 O5 1_554 . -11.1(4) no
Dy1 O4 B2 Dy2 2_766 . -60.9(9) no
Dy2 O4 B2 Dy2 1_655 . 154.9(6) no
Dy1 O4 B2 Dy2 1_554 . 50.0(8) no
Dy1 O4 B2 Dy1 2_766 1_554 -110.9(3) no
Dy2 O4 B2 Dy1 1_655 1_554 104.9(3) no
Dy2 O5 B2 O6 . . -25.3(5) no
Dy1 O5 B2 O6 2_776 . 80.6(5) no
Dy1 O5 B2 O6 1_554 . -165.3(4) no
Dy2 O5 B2 O4 . . 151.4(4) no
Dy1 O5 B2 O4 2_776 . -102.7(4) no
Dy1 O5 B2 O4 1_554 . 11.4(4) no
Dy1 O5 B2 Dy2 2_776 . 105.9(2) no
Dy1 O5 B2 Dy2 1_554 . -139.97(19) no
Dy2 O5 B2 Dy1 . 1_554 139.97(19) no
Dy1 O5 B2 Dy1 2_776 1_554 -114.2(2) no
O2 Dy2 B2 O6 2_666 . -83.0(3) no
O1 Dy2 B2 O6 . . 6.5(3) no
O5 Dy2 B2 O6 . . 155.8(5) no
O1 Dy2 B2 O6 2_676 . 82.9(4) no
O3 Dy2 B2 O6 1_554 . -163.9(3) no
O4 Dy2 B2 O6 1_455 . -90.4(3) no
O3 Dy2 B2 O6 2_676 . 124.5(3) no
B1 Dy2 B2 O6 2_676 . 107.9(3) no
Dy1 Dy2 B2 O6 2_776 . 114.8(3) no
Dy2 Dy2 B2 O6 2_676 . 35.2(4) no
O2 Dy2 B2 O4 2_666 . 45.5(8) no
O1 Dy2 B2 O4 . . 135.0(8) no
O5 Dy2 B2 O4 . . -75.7(8) no
O1 Dy2 B2 O4 2_676 . -148.6(8) no
O3 Dy2 B2 O4 1_554 . -35.4(9) no
O4 Dy2 B2 O4 1_455 . 38.1(9) no
O3 Dy2 B2 O4 2_676 . -107.0(8) no
O6 Dy2 B2 O4 . . 128.5(10) no
B1 Dy2 B2 O4 2_676 . -123.6(8) no
Dy1 Dy2 B2 O4 2_776 . -116.7(9) no
Dy2 Dy2 B2 O4 2_676 . 163.7(8) no
O2 Dy2 B2 O5 2_666 . 121.1(3) no
O1 Dy2 B2 O5 . . -149.3(2) no
O1 Dy2 B2 O5 2_676 . -72.9(3) no
O3 Dy2 B2 O5 1_554 . 40.3(3) no
O4 Dy2 B2 O5 1_455 . 113.7(3) no
O3 Dy2 B2 O5 2_676 . -31.3(3) no
O6 Dy2 B2 O5 . . -155.8(5) no
B1 Dy2 B2 O5 2_676 . -47.9(3) no
Dy1 Dy2 B2 O5 2_776 . -41.0(2) no
Dy2 Dy2 B2 O5 2_676 . -120.6(2) no
O2 Dy2 B2 Dy1 2_666 1_554 87.83(17) no
O1 Dy2 B2 Dy1 . 1_554 177.36(14) no
O5 Dy2 B2 Dy1 . 1_554 -33.3(2) no
O1 Dy2 B2 Dy1 2_676 1_554 -106.2(2) no
O3 Dy2 B2 Dy1 1_554 1_554 6.95(18) no
O4 Dy2 B2 Dy1 1_455 1_554 80.4(3) no
O3 Dy2 B2 Dy1 2_676 1_554 -64.61(16) no
O6 Dy2 B2 Dy1 . 1_554 170.9(4) no
B1 Dy2 B2 Dy1 2_676 1_554 -81.22(19) no
Dy1 Dy2 B2 Dy1 2_776 1_554 -74.32(15) no
Dy2 Dy2 B2 Dy1 2_676 1_554 -153.96(7) no
